#------------------------------------------------------------------------------
#$Date: 2016-03-23 23:55:35 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179518 $
#$URL: svn://www.crystallography.net/cod/cif/4/34/15/4341581.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4341581
loop_
_publ_author_name
'Ren, Yi-Xia'
'Zheng, Xiang-Jun'
'Li, Li-Cun'
'Yuan, Da-Qiang'
'An, Miao'
'Jin, Lin-Pei'
_publ_section_title
;
 Three-Dimensional Frameworks Based on Dodecanuclear Dy-hydroxo Wheel
 Cluster with Slow Relaxation of Magnetization.
;
_journal_name_full               'Inorganic chemistry'
_journal_page_first              141113084659009
_journal_paper_doi               10.1021/ic502042h
_journal_year                    2014
_chemical_formula_sum            'C32 H42 Ho6 Na2 O47 S4'
_chemical_formula_weight         2342.45
_chemical_name_systematic
;
 ?
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           12
_space_group_name_Hall           '-C 2y'
_space_group_name_H-M_alt        'C 1 2/m 1'
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_hydrogens   mixed
_audit_creation_method           SHELXL-2014
_cell_angle_alpha                90
_cell_angle_beta                 118.719(5)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   26.781(8)
_cell_length_b                   17.916(5)
_cell_length_c                   13.763(4)
_cell_measurement_reflns_used    1389
_cell_measurement_temperature    110(2)
_cell_measurement_theta_max      23.959
_cell_measurement_theta_min      2.5865
_cell_volume                     5791(3)
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      110(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.978
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1114
_diffrn_reflns_av_unetI/netI     0.1533
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.978
_diffrn_reflns_limit_h_max       34
_diffrn_reflns_limit_h_min       -27
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_k_min       -23
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            17198
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.978
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.741
_diffrn_reflns_theta_min         2.586
_diffrn_source                   'fine-focus sealed tube'
_exptl_absorpt_coefficient_mu    8.377
_exptl_absorpt_correction_T_max  0.7305
_exptl_absorpt_correction_T_min  0.6334
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   sadabs
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    2.687
_exptl_crystal_description       block
_exptl_crystal_F_000             4392
_exptl_crystal_size_max          0.060
_exptl_crystal_size_mid          0.050
_exptl_crystal_size_min          0.040
_refine_diff_density_max         3.416
_refine_diff_density_min         -3.389
_refine_diff_density_rms         0.413
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.012
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     403
_refine_ls_number_reflns         6887
_refine_ls_number_restraints     66
_refine_ls_restrained_S_all      1.010
_refine_ls_R_factor_all          0.1431
_refine_ls_R_factor_gt           0.0745
_refine_ls_shift/su_max          0.013
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0897P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1695
_refine_ls_wR_factor_ref         0.2014
_reflns_Friedel_coverage         0.000
_reflns_number_gt                3832
_reflns_number_total             6887
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            ic502042h_si_002.cif
_cod_data_source_block           Ho
_cod_original_cell_volume        5792(3)
_cod_database_code               4341581
#BEGIN Tags that were not found in dictionaries:
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.633
_shelx_estimated_absorpt_t_max   0.731
_shelxl_version_number           2014-3
#END Tags that were not found in dictionaries
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
Ho1 Ho 0.47832(5) 1.0000 0.34105(10) 0.0183(3) Uani 1 2 d S T P
Ho2 Ho 0.63237(4) 1.0000 0.41109(9) 0.0166(3) Uani 1 2 d S T P
Ho3 Ho 0.52261(3) 0.89623(5) 0.15804(6) 0.0170(2) Uani 1 1 d . . .
Ho4 Ho 0.57756(3) 0.76585(6) 0.03623(7) 0.0292(3) Uani 1 1 d . . .
S1 S 0.5800(2) 0.6655(3) -0.1802(5) 0.0357(13) Uani 1 1 d . . .
S2 S 0.6403(2) 0.6644(3) 0.2862(4) 0.0311(12) Uani 1 1 d . . .
Na1 Na 0.6288(6) 0.5000 0.1683(12) 0.074(5) Uani 1 2 d S T P
Na2 Na 0.8637(7) 0.5000 -0.0527(17) 0.089(6) Uani 1 2 d S T P
O1 O 0.8514(5) 0.5824(7) 0.4442(9) 0.021(3) Uani 1 1 d . . .
O2 O 0.9064(6) 0.6797(8) 0.4827(12) 0.040(4) Uani 1 1 d . U .
O3 O 0.6700(5) 0.8985(8) 0.3716(9) 0.029(3) Uani 1 1 d . . .
O4 O 0.6150(5) 0.8315(7) 0.2225(10) 0.027(3) Uani 1 1 d . . .
O5 O 0.6141(5) 0.6689(7) 0.1626(11) 0.033(3) Uani 1 1 d . . .
O6 O 0.6556(6) 0.5883(8) 0.3187(13) 0.050(4) Uani 1 1 d . . .
O7 O 0.6064(5) 0.7001(9) 0.3298(12) 0.040(4) Uani 1 1 d . . .
O8 O 0.5732(5) 0.8919(8) -0.2723(10) 0.028(3) Uani 1 1 d . U .
O9 O 0.5638(5) 0.8349(7) -0.1379(10) 0.028(3) Uani 1 1 d . U .
O10 O 0.8330(5) 0.7067(7) -0.0800(10) 0.028(3) Uani 1 1 d . U .
O11 O 0.7857(6) 0.6024(8) -0.0958(13) 0.046(4) Uani 1 1 d . . .
O12 O 0.5290(5) 0.7007(8) -0.2665(11) 0.039(4) Uani 1 1 d . . .
O13 O 0.5895(6) 0.5900(9) -0.2036(15) 0.058(5) Uani 1 1 d . . .
O14 O 0.5830(5) 0.6710(7) -0.0733(12) 0.035(3) Uani 1 1 d . . .
O15 O 0.5517(4) 0.8907(7) 0.0224(8) 0.019(3) Uani 1 1 d . . .
H15 H 0.5774 0.9229 0.0347 0.023 Uiso 1 1 d R U .
O16 O 0.5145(5) 0.7719(7) 0.1058(10) 0.024(3) Uani 1 1 d . . .
H16 H 0.5207 0.7373 0.1525 0.029 Uiso 1 1 d R U .
O17 O 0.5831(6) 1.0000 0.2099(12) 0.013(3) Uani 1 2 d S TU P
H17 H 0.6052 1.0000 0.1816 0.016 Uiso 1 2 d R U P
O18 O 0.5500(4) 0.9224(6) 0.3412(9) 0.017(2) Uani 1 1 d . U .
H18 H 0.5564 0.8838 0.3814 0.021 Uiso 1 1 d R U .
O19 O 0.4707(7) 1.0000 0.1607(13) 0.022(4) Uani 1 2 d S T P
H19 H 0.4372 1.0000 0.1062 0.027 Uiso 1 2 d R U P
O20 O 0.7379(7) 1.0000 0.5220(15) 0.035(5) Uani 1 2 d S T P
H20 H 0.7588 0.9641 0.5227 0.042 Uiso 1 1 d R U .
O21 O 0.5000 0.9214(18) 0.5000 0.087(4) Uani 1 2 d S T P
H21 H 0.5289 0.8946 0.5137 0.105 Uiso 1 1 d R U .
O22 O 0.3823(10) 1.0000 0.320(2) 0.087(4) Uani 1 2 d S T P
H22 H 0.3745 0.9616 0.3465 0.105 Uiso 1 1 d R U .
O23 O 0.5349(10) 0.5000 0.154(2) 0.087(4) Uani 1 2 d S T P
H23 H 0.5362 0.5410 0.1864 0.105 Uiso 1 1 d R U .
O24 O 0.7240(11) 0.5000 0.202(2) 0.087(4) Uani 1 2 d S T P
H24A H 0.7335 0.5000 0.1513 0.105 Uiso 1 2 d R U P
H24B H 0.7542 0.5000 0.2644 0.105 Uiso 1 2 d R U P
O25 O 0.5878(10) 0.5000 -0.019(2) 0.087(4) Uani 1 2 d S T P
H25 H 0.5878 0.5385 -0.0547 0.105 Uiso 1 1 d R U .
O26 O 0.7564(16) 1.0000 -0.018(3) 0.143(7) Uani 1 2 d S T P
H26 H 0.7459 1.0376 0.0048 0.172 Uiso 1 1 d R U .
O27 O 0.4688(17) 0.5000 -0.339(3) 0.143(7) Uani 1 2 d S T P
H27 H 0.4911 0.5368 -0.3097 0.172 Uiso 1 1 d R U .
O28 O 0.7190(16) 0.5000 -0.276(3) 0.143(7) Uani 1 2 d S T P
H28 H 0.7296 0.5392 -0.2369 0.172 Uiso 1 1 d R U .
O29 O 0.452(2) 0.704(3) -0.430(4) 0.143(7) Uani 0.5 1 d . . P
H29A H 0.4839 0.7106 -0.3716 0.172 Uiso 0.5 1 d R U P
H29B H 0.4416 0.7470 -0.4593 0.172 Uiso 0.5 1 d R U P
O30 O 0.5000 0.641(2) 0.0000 0.143(7) Uani 1 2 d S T P
H30 H 0.5290 0.6160 0.0440 0.172 Uiso 1 1 d R U .
C1 C 0.8108(8) 0.7774(11) 0.4121(14) 0.026(4) Uani 1 1 d . U .
H1 H 0.8470 0.8002 0.4377 0.031 Uiso 1 1 calc R U .
C2 C 0.7642(7) 0.8229(11) 0.3799(14) 0.024(4) Uani 1 1 d . . .
H2 H 0.7683 0.8756 0.3835 0.028 Uiso 1 1 calc R U .
C3 C 0.7108(7) 0.7905(11) 0.3420(13) 0.023(4) Uani 1 1 d . . .
C4 C 0.7052(7) 0.7132(10) 0.3347(14) 0.018(4) Uani 1 1 d . . .
C5 C 0.7553(7) 0.6690(11) 0.3702(14) 0.026(4) Uani 1 1 d . . .
H5 H 0.7521 0.6162 0.3668 0.031 Uiso 1 1 calc R U .
C6 C 0.8081(7) 0.7015(11) 0.4095(14) 0.025(4) Uani 1 1 d . . .
C7 C 0.8589(7) 0.6519(11) 0.4458(15) 0.025(4) Uani 1 1 d . . .
C8 C 0.6616(8) 0.8412(12) 0.3085(15) 0.027(4) Uani 1 1 d . . .
C9 C 0.7376(8) 0.7168(11) -0.1281(15) 0.024(4) Uani 1 1 d . U .
C10 C 0.6876(7) 0.6803(12) -0.1431(16) 0.030(5) Uani 1 1 d . . .
H10 H 0.6883 0.6277 -0.1337 0.036 Uiso 1 1 calc R U .
C11 C 0.6385(7) 0.7178(11) -0.1703(16) 0.027(5) Uani 1 1 d . . .
C12 C 0.6387(7) 0.7947(10) -0.1756(14) 0.019(4) Uani 1 1 d . . .
C13 C 0.6866(7) 0.8325(10) -0.1627(14) 0.020(4) Uani 1 1 d . . .
H13 H 0.6859 0.8853 -0.1707 0.025 Uiso 1 1 calc R U .
C14 C 0.7361(7) 0.7922(9) -0.1377(13) 0.017(4) Uani 1 1 d . U .
H14 H 0.7693 0.8181 -0.1273 0.020 Uiso 1 1 calc R U .
C15 C 0.7896(7) 0.6723(11) -0.1006(14) 0.023(4) Uani 1 1 d . U .
C16 C 0.5868(8) 0.8431(12) -0.1995(16) 0.030(4) Uani 1 1 d . U .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
S S 0.1246 0.1234 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ho Ho -0.2175 4.6783 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O8 Ho1 O8 114.6(6) 2_655 5_675
O8 Ho1 O18 145.0(4) 2_655 6_575
O8 Ho1 O18 80.3(4) 5_675 6_575
O8 Ho1 O18 80.3(4) 2_655 .
O8 Ho1 O18 145.0(4) 5_675 .
O18 Ho1 O18 71.8(5) 6_575 .
O8 Ho1 O19 80.7(3) 2_655 .
O8 Ho1 O19 80.7(3) 5_675 .
O18 Ho1 O19 70.4(4) 6_575 .
O18 Ho1 O19 70.4(4) . .
O8 Ho1 O21 134.1(6) 2_655 5_676
O8 Ho1 O21 73.7(6) 5_675 5_676
O18 Ho1 O21 79.4(5) 6_575 5_676
O18 Ho1 O21 119.8(4) . 5_676
O19 Ho1 O21 143.2(6) . 5_676
O8 Ho1 O21 73.7(6) 2_655 .
O8 Ho1 O21 134.1(6) 5_675 .
O18 Ho1 O21 119.8(4) 6_575 .
O18 Ho1 O21 79.4(5) . .
O19 Ho1 O21 143.1(6) . .
O21 Ho1 O21 71.0(13) 5_676 .
O8 Ho1 O22 64.1(4) 2_655 .
O8 Ho1 O22 64.1(4) 5_675 .
O18 Ho1 O22 143.7(3) 6_575 .
O18 Ho1 O22 143.7(3) . .
O19 Ho1 O22 108.5(7) . .
O21 Ho1 O22 83.6(5) 5_676 .
O21 Ho1 O22 83.6(5) . .
O8 Ho1 Ho3 68.1(3) 2_655 .
O8 Ho1 Ho3 117.5(3) 5_675 .
O18 Ho1 Ho3 76.9(3) 6_575 .
O18 Ho1 Ho3 36.1(3) . .
O19 Ho1 Ho3 36.8(2) . .
O21 Ho1 Ho3 151.29(5) 5_676 .
O21 Ho1 Ho3 107.6(5) . .
O22 Ho1 Ho3 125.0(5) . .
O8 Ho1 Ho3 117.5(3) 2_655 6_575
O8 Ho1 Ho3 68.1(3) 5_675 6_575
O18 Ho1 Ho3 36.1(3) 6_575 6_575
O18 Ho1 Ho3 76.9(3) . 6_575
O19 Ho1 Ho3 36.8(2) . 6_575
O21 Ho1 Ho3 107.6(6) 5_676 6_575
O21 Ho1 Ho3 151.29(5) . 6_575
O22 Ho1 Ho3 125.0(5) . 6_575
Ho3 Ho1 Ho3 59.40(4) . 6_575
O8 Ho1 Ho2 118.2(3) 2_655 .
O8 Ho1 Ho2 118.2(3) 5_675 .
O18 Ho1 Ho2 37.9(3) 6_575 .
O18 Ho1 Ho2 37.9(3) . .
O19 Ho1 Ho2 78.5(4) . .
O21 Ho1 Ho2 90.64(3) 5_676 .
O21 Ho1 Ho2 90.64(3) . .
O22 Ho1 Ho2 173.0(6) . .
Ho3 Ho1 Ho2 60.67(3) . .
Ho3 Ho1 Ho2 60.66(3) 6_575 .
O8 Ho1 Ho1 104.8(3) 2_655 5_676
O8 Ho1 Ho1 104.8(3) 5_675 5_676
O18 Ho1 Ho1 101.1(3) 6_575 5_676
O18 Ho1 Ho1 101.1(3) . 5_676
O19 Ho1 Ho1 169.3(4) . 5_676
O21 Ho1 Ho1 35.5(6) 5_676 5_676
O21 Ho1 Ho1 35.5(6) . 5_676
O22 Ho1 Ho1 82.2(6) . 5_676
Ho3 Ho1 Ho1 136.38(4) . 5_676
Ho3 Ho1 Ho1 136.38(4) 6_575 5_676
Ho2 Ho1 Ho1 90.78(4) . 5_676
O3 Ho2 O3 106.6(7) . 6_575
O3 Ho2 O1 141.8(4) . 4_656
O3 Ho2 O1 77.1(4) 6_575 4_656
O3 Ho2 O1 77.1(4) . 7_666
O3 Ho2 O1 141.8(4) 6_575 7_666
O1 Ho2 O1 78.0(6) 4_656 7_666
O3 Ho2 O18 82.4(4) . .
O3 Ho2 O18 143.3(4) 6_575 .
O1 Ho2 O18 117.9(4) 4_656 .
O1 Ho2 O18 74.5(4) 7_666 .
O3 Ho2 O18 143.3(4) . 6_575
O3 Ho2 O18 82.4(4) 6_575 6_575
O1 Ho2 O18 74.5(4) 4_656 6_575
O1 Ho2 O18 117.9(4) 7_666 6_575
O18 Ho2 O18 71.3(5) . 6_575
O3 Ho2 O17 77.7(3) . .
O3 Ho2 O17 77.7(3) 6_575 .
O1 Ho2 O17 138.2(3) 4_656 .
O1 Ho2 O17 138.2(3) 7_666 .
O18 Ho2 O17 69.5(4) . .
O18 Ho2 O17 69.5(4) 6_575 .
O3 Ho2 O20 69.0(4) . .
O3 Ho2 O20 69.0(4) 6_575 .
O1 Ho2 O20 77.7(4) 4_656 .
O1 Ho2 O20 77.7(4) 7_666 .
O18 Ho2 O20 143.8(3) . .
O18 Ho2 O20 143.8(3) 6_575 .
O17 Ho2 O20 122.3(5) . .
O3 Ho2 Ho1 119.9(3) . .
O3 Ho2 Ho1 119.9(3) 6_575 .
O1 Ho2 Ho1 87.1(3) 4_656 .
O1 Ho2 Ho1 87.1(3) 7_666 .
O18 Ho2 Ho1 37.6(3) . .
O18 Ho2 Ho1 37.6(3) 6_575 .
O17 Ho2 Ho1 77.3(3) . .
O20 Ho2 Ho1 160.4(4) . .
O3 Ho2 Ho3 114.2(3) . 6_575
O3 Ho2 Ho3 68.0(3) 6_575 6_575
O1 Ho2 Ho3 102.5(3) 4_656 6_575
O1 Ho2 Ho3 146.5(3) 7_666 6_575
O18 Ho2 Ho3 75.9(3) . 6_575
O18 Ho2 Ho3 35.4(3) 6_575 6_575
O17 Ho2 Ho3 36.5(2) . 6_575
O20 Ho2 Ho3 135.7(3) . 6_575
Ho1 Ho2 Ho3 59.58(3) . 6_575
O3 Ho2 Ho3 68.0(3) . .
O3 Ho2 Ho3 114.2(3) 6_575 .
O1 Ho2 Ho3 146.5(3) 4_656 .
O1 Ho2 Ho3 102.5(3) 7_666 .
O18 Ho2 Ho3 35.4(3) . .
O18 Ho2 Ho3 75.9(3) 6_575 .
O17 Ho2 Ho3 36.5(2) . .
O20 Ho2 Ho3 135.7(3) . .
Ho1 Ho2 Ho3 59.58(3) . .
Ho3 Ho2 Ho3 58.70(3) 6_575 .
O18 Ho3 O16 117.8(4) . .
O18 Ho3 O15 146.7(4) . 2_655
O16 Ho3 O15 73.9(4) . 2_655
O18 Ho3 O19 72.6(5) . .
O16 Ho3 O19 143.4(4) . .
O15 Ho3 O19 80.8(5) 2_655 .
O18 Ho3 O17 72.3(5) . .
O16 Ho3 O17 143.7(4) . .
O15 Ho3 O17 118.2(4) 2_655 .
O19 Ho3 O17 72.1(4) . .
O18 Ho3 O15 145.5(4) . .
O16 Ho3 O15 74.3(4) . .
O15 Ho3 O15 65.7(4) 2_655 .
O19 Ho3 O15 118.3(5) . .
O17 Ho3 O15 80.2(5) . .
O18 Ho3 O9 90.1(4) . 2_655
O16 Ho3 O9 65.9(4) . 2_655
O15 Ho3 O9 65.3(4) 2_655 2_655
O19 Ho3 O9 79.8(4) . 2_655
O17 Ho3 O9 150.1(4) . 2_655
O15 Ho3 O9 123.2(4) . 2_655
O18 Ho3 O4 88.0(4) . .
O16 Ho3 O4 65.8(4) . .
O15 Ho3 O4 123.9(4) 2_655 .
O19 Ho3 O4 150.1(5) . .
O17 Ho3 O4 80.6(4) . .
O15 Ho3 O4 67.0(4) . .
O9 Ho3 O4 123.8(4) 2_655 .
O18 Ho3 Ho4 131.1(3) . .
O16 Ho3 Ho4 39.3(3) . .
O15 Ho3 Ho4 78.8(3) 2_655 .
O19 Ho3 Ho4 155.5(4) . .
O17 Ho3 Ho4 106.3(3) . .
O15 Ho3 Ho4 39.7(3) . .
O9 Ho3 Ho4 103.4(3) 2_655 .
O4 Ho3 Ho4 45.4(3) . .
O18 Ho3 Ho4 132.6(3) . 2_655
O16 Ho3 Ho4 38.7(3) . 2_655
O15 Ho3 Ho4 39.3(3) 2_655 2_655
O19 Ho3 Ho4 107.0(3) . 2_655
O17 Ho3 Ho4 154.6(4) . 2_655
O15 Ho3 Ho4 78.2(3) . 2_655
O9 Ho3 Ho4 45.5(3) 2_655 2_655
O4 Ho3 Ho4 102.8(3) . 2_655
Ho4 Ho3 Ho4 63.58(4) . 2_655
O18 Ho3 Ho3 78.3(3) . 6_575
O16 Ho3 Ho3 163.9(3) . 6_575
O15 Ho3 Ho3 92.5(3) 2_655 6_575
O19 Ho3 Ho3 37.1(3) . 6_575
O17 Ho3 Ho3 37.4(3) . 6_575
O15 Ho3 Ho3 92.4(3) . 6_575
O9 Ho3 Ho3 116.6(3) 2_655 6_575
O4 Ho3 Ho3 117.9(3) . 6_575
Ho4 Ho3 Ho3 130.75(2) . 6_575
Ho4 Ho3 Ho3 130.55(2) 2_655 6_575
O18 Ho3 Ho1 37.2(3) . .
O16 Ho3 Ho1 132.1(3) . .
O15 Ho3 Ho1 110.7(3) 2_655 .
O19 Ho3 Ho1 38.0(4) . .
O17 Ho3 Ho1 78.3(3) . .
O15 Ho3 Ho1 152.7(3) . .
O9 Ho3 Ho1 73.3(3) 2_655 .
O4 Ho3 Ho1 125.1(3) . .
Ho4 Ho3 Ho1 166.36(3) . .
Ho4 Ho3 Ho1 117.25(3) 2_655 .
Ho3 Ho3 Ho1 60.299(17) 6_575 .
O10 Ho4 O16 142.6(4) 7_665 2_655
O10 Ho4 O16 141.6(4) 7_665 .
O16 Ho4 O16 69.6(5) 2_655 .
O10 Ho4 O5 87.2(4) 7_665 .
O16 Ho4 O5 124.6(4) 2_655 .
O16 Ho4 O5 81.5(4) . .
O10 Ho4 O15 92.8(4) 7_665 .
O16 Ho4 O15 74.3(4) 2_655 .
O16 Ho4 O15 75.0(4) . .
O5 Ho4 O15 141.8(4) . .
O10 Ho4 O14 86.7(4) 7_665 .
O16 Ho4 O14 81.8(4) 2_655 .
O16 Ho4 O14 126.1(4) . .
O5 Ho4 O14 78.7(5) . .
O15 Ho4 O14 139.5(4) . .
O10 Ho4 O4 76.9(4) 7_665 .
O16 Ho4 O4 125.3(4) 2_655 .
O16 Ho4 O4 64.8(4) . .
O5 Ho4 O4 76.7(4) . .
O15 Ho4 O4 66.2(4) . .
O14 Ho4 O4 150.9(4) . .
O10 Ho4 O9 78.4(4) 7_665 .
O16 Ho4 O9 64.4(4) 2_655 .
O16 Ho4 O9 124.1(4) . .
O5 Ho4 O9 152.1(4) . .
O15 Ho4 O9 63.5(4) . .
O14 Ho4 O9 76.8(4) . .
O4 Ho4 O9 121.9(4) . .
O10 Ho4 Ho3 111.1(3) 7_665 .
O16 Ho4 Ho3 81.6(3) 2_655 .
O16 Ho4 Ho3 39.5(3) . .
O5 Ho4 Ho3 105.0(3) . .
O15 Ho4 Ho3 40.2(2) . .
O14 Ho4 Ho3 161.8(3) . .
O4 Ho4 Ho3 43.9(3) . .
O9 Ho4 Ho3 102.5(3) . .
O10 Ho4 Ho3 112.3(3) 7_665 2_655
O16 Ho4 Ho3 39.1(3) 2_655 2_655
O16 Ho4 Ho3 81.1(3) . 2_655
O5 Ho4 Ho3 160.3(3) . 2_655
O15 Ho4 Ho3 39.3(2) . 2_655
O14 Ho4 Ho3 104.5(3) . 2_655
O4 Ho4 Ho3 103.9(3) . 2_655
O9 Ho4 Ho3 43.0(3) . 2_655
Ho3 Ho4 Ho3 66.18(3) . 2_655
O10 Ho4 Ho4 167.2(3) 7_665 2_655
O16 Ho4 Ho4 35.1(3) 2_655 2_655
O16 Ho4 Ho4 34.8(3) . 2_655
O5 Ho4 Ho4 102.3(3) . 2_655
O15 Ho4 Ho4 74.4(3) . 2_655
O14 Ho4 Ho4 103.5(3) . 2_655
O4 Ho4 Ho4 96.7(3) . 2_655
O9 Ho4 Ho4 96.2(3) . 2_655
Ho3 Ho4 Ho4 58.40(2) . 2_655
Ho3 Ho4 Ho4 58.02(2) 2_655 2_655
O14 S1 O13 111.4(10) . .
O14 S1 O12 111.9(8) . .
O13 S1 O12 115.0(9) . .
O14 S1 C11 105.8(8) . .
O13 S1 C11 105.5(9) . .
O12 S1 C11 106.4(9) . .
O6 S2 O7 115.5(9) . .
O6 S2 O5 108.3(9) . .
O7 S2 O5 113.5(8) . .
O6 S2 C4 105.8(8) . .
O7 S2 C4 108.8(8) . .
O5 S2 C4 104.0(7) . .
O7 S2 Na1 131.6(7) . .
O5 S2 Na1 67.0(6) . .
C4 S2 Na1 118.0(6) . .
O25 Na1 O24 96.4(10) . .
O25 Na1 O6 139.0(4) . 6_565
O24 Na1 O6 89.1(7) . 6_565
O25 Na1 O6 139.0(4) . .
O24 Na1 O6 89.1(7) . .
O6 Na1 O6 81.5(8) 6_565 .
O25 Na1 O23 89.5(10) . .
O24 Na1 O23 174.1(11) . .
O6 Na1 O23 86.4(7) 6_565 .
O6 Na1 O23 86.4(7) . .
O25 Na1 S2 116.0(3) . .
O24 Na1 S2 93.8(4) . .
O6 Na1 S2 104.1(6) 6_565 .
O6 Na1 S2 23.0(4) . .
O23 Na1 S2 83.6(4) . .
O25 Na1 S2 116.0(3) . 6_565
O24 Na1 S2 93.8(4) . 6_565
O6 Na1 S2 23.0(4) 6_565 6_565
O6 Na1 S2 104.1(6) . 6_565
O23 Na1 S2 83.6(4) . 6_565
S2 Na1 S2 126.1(5) . 6_565
O11 Na2 O11 88.6(8) 6_565 .
O11 Na2 O15 175.5(9) 6_565 7_665
O11 Na2 O15 92.5(4) . 7_665
O11 Na2 O15 92.5(4) 6_565 4_645
O11 Na2 O15 175.5(9) . 4_645
O15 Na2 O15 86.1(6) 7_665 4_645
O11 Na2 O19 120.7(7) 6_565 3_545
O11 Na2 O19 120.7(7) . 3_545
O15 Na2 O19 62.3(4) 7_665 3_545
O15 Na2 O19 62.3(4) 4_645 3_545
C7 O1 Ho2 130.1(11) . 7_666
C8 O3 Ho2 147.5(11) . .
C8 O4 Ho3 130.0(13) . .
C8 O4 Ho4 138.4(12) . .
Ho3 O4 Ho4 90.7(4) . .
S2 O5 Ho4 133.8(8) . .
S2 O6 Na1 115.6(9) . .
C16 O8 Ho1 143.9(12) . 5_675
C16 O9 Ho3 127.3(12) . 2_655
C16 O9 Ho4 141.2(12) . .
Ho3 O9 Ho4 91.5(4) 2_655 .
C15 O10 Ho4 162.5(13) . 7_665
C15 O11 Na2 129.0(12) . .
S1 O12 H29A 156.5 . .
S1 O14 Ho4 136.4(8) . .
Ho4 O15 Ho3 101.4(4) . 2_655
Ho4 O15 Ho3 100.1(4) . .
Ho3 O15 Ho3 114.0(4) 2_655 .
Ho4 O15 Na2 117.6(4) . 7_665
Ho3 O15 Na2 109.7(5) 2_655 7_665
Ho3 O15 Na2 113.3(6) . 7_665
Ho4 O15 H15 117.3 . .
Ho3 O15 H15 112.3 2_655 .
Ho3 O15 H15 110.9 . .
Ho4 O16 Ho4 110.1(5) 2_655 .
Ho4 O16 Ho3 102.2(5) 2_655 .
Ho4 O16 Ho3 101.2(4) . .
Ho4 O16 H16 110.4 2_655 .
Ho4 O16 H16 111.3 . .
Ho3 O16 H16 120.7 . .
Ho3 O17 Ho3 105.1(6) 6_575 .
Ho3 O17 Ho2 105.4(4) 6_575 .
Ho3 O17 Ho2 105.4(4) . .
Ho3 O17 H17 113.1 6_575 .
Ho3 O17 H17 113.1 . .
Ho2 O17 H17 114.0 . .
Ho3 O18 Ho1 106.6(4) . .
Ho3 O18 Ho2 107.8(4) . .
Ho1 O18 Ho2 104.5(4) . .
Ho3 O18 H18 113.8 . .
Ho1 O18 H18 112.8 . .
Ho2 O18 H18 110.7 . .
Ho3 O19 Ho3 105.8(6) . 6_575
Ho3 O19 Ho1 105.2(5) . .
Ho3 O19 Ho1 105.2(5) 6_575 .
Ho3 O19 Na2 106.6(5) . 3_455
Ho3 O19 Na2 106.6(5) 6_575 3_455
Ho1 O19 Na2 126.1(7) . 3_455
Ho3 O19 H19 111.8 . .
Ho3 O19 H19 111.8 6_575 .
Ho1 O19 H19 116.2 . .
Ho2 O20 H20 123.8 . .
Ho1 O21 Ho1 109.0(13) 5_676 .
Ho1 O21 H21 109.2 5_676 .
Ho1 O21 H21 109.1 . .
Ho1 O22 H22 114.2 . .
Na1 O23 H23 100.3 . .
Na1 O24 H24A 124.0 . .
Na1 O24 H24B 127.7 . .
H24A O24 H24B 108.4 . .
Na1 O25 H25 121.9 . .
H29A O29 H29B 106.3 . .
C6 C1 C2 123.8(18) . .
C6 C1 H1 118.1 . .
C2 C1 H1 118.1 . .
C1 C2 C3 119.0(18) . .
C1 C2 H2 120.5 . .
C3 C2 H2 120.5 . .
C4 C3 C2 119.8(16) . .
C4 C3 C8 122.7(16) . .
C2 C3 C8 117.5(17) . .
C3 C4 C5 118.5(16) . .
C3 C4 S2 124.9(13) . .
C5 C4 S2 116.6(13) . .
C6 C5 C4 121.3(18) . .
C6 C5 H5 119.3 . .
C4 C5 H5 119.3 . .
C1 C6 C5 117.6(18) . .
C1 C6 C7 123.9(17) . .
C5 C6 C7 118.6(18) . .
O2 C7 O1 122.2(16) . .
O2 C7 C6 119.5(18) . .
O1 C7 C6 118.1(16) . .
O4 C8 O3 121.2(17) . .
O4 C8 C3 122.8(18) . .
O3 C8 C3 115.9(16) . .
C14 C9 C10 117.8(17) . .
C14 C9 C15 122.6(16) . .
C10 C9 C15 119.6(17) . .
C11 C10 C9 122.3(19) . .
C11 C10 H10 118.9 . .
C9 C10 H10 118.9 . .
C10 C11 C12 118.8(17) . .
C10 C11 S1 117.5(16) . .
C12 C11 S1 123.3(13) . .
C11 C12 C13 120.6(15) . .
C11 C12 C16 123.3(15) . .
C13 C12 C16 116.1(16) . .
C12 C13 C14 119.2(16) . .
C12 C13 H13 120.4 . .
C14 C13 H13 120.4 . .
C9 C14 C13 121.2(16) . .
C9 C14 H14 119.4 . .
C13 C14 H14 119.4 . .
O10 C15 O11 125.6(17) . .
O10 C15 C9 117.2(17) . .
O11 C15 C9 117.1(16) . .
O8 C16 O9 124.6(18) . .
O8 C16 C12 117.0(16) . .
O9 C16 C12 118.2(17) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ho1 O8 2.301(13) 2_655
Ho1 O8 2.301(13) 5_675
Ho1 O18 2.370(10) 6_575
Ho1 O18 2.370(10) .
Ho1 O19 2.392(16) .
Ho1 O21 2.426(19) 5_676
Ho1 O21 2.426(19) .
Ho1 O22 2.45(2) .
Ho1 Ho3 3.7521(14) .
Ho1 Ho3 3.7521(14) 6_575
Ho1 Ho2 3.7588(19) .
Ho1 Ho1 3.951(3) 5_676
Ho2 O3 2.268(13) .
Ho2 O3 2.268(13) 6_575
Ho2 O1 2.346(11) 4_656
Ho2 O1 2.346(11) 7_666
Ho2 O18 2.384(11) .
Ho2 O18 2.384(11) 6_575
Ho2 O17 2.428(14) .
Ho2 O20 2.483(16) .
Ho2 Ho3 3.7931(14) 6_575
Ho2 Ho3 3.7932(14) .
Ho3 O18 2.310(11) .
Ho3 O16 2.319(12) .
Ho3 O15 2.321(10) 2_655
Ho3 O19 2.331(10) .
Ho3 O17 2.341(9) .
Ho3 O15 2.346(10) .
Ho3 O9 2.453(12) 2_655
Ho3 O4 2.480(12) .
Ho3 Ho4 3.5784(13) .
Ho3 Ho4 3.5930(13) 2_655
Ho3 Ho3 3.718(2) 6_575
Ho4 O10 2.227(12) 7_665
Ho4 O16 2.297(12) 2_655
Ho4 O16 2.311(11) .
Ho4 O5 2.316(13) .
Ho4 O15 2.321(12) .
Ho4 O14 2.322(14) .
Ho4 O4 2.548(13) .
Ho4 O9 2.561(12) .
Ho4 Ho3 3.5931(13) 2_655
Ho4 Ho4 3.778(2) 2_655
S1 O14 1.438(15) .
S1 O13 1.440(16) .
S1 O12 1.456(15) .
S1 C11 1.775(18) .
S2 O6 1.433(16) .
S2 O7 1.456(13) .
S2 O5 1.498(14) .
S2 C4 1.764(17) .
S2 Na1 3.305(9) .
Na1 O25 2.26(3) .
Na1 O24 2.36(3) .
Na1 O6 2.42(2) 6_565
Na1 O6 2.42(2) .
Na1 O23 2.43(3) .
Na1 S2 3.305(9) 6_565
Na2 O11 2.625(17) 6_565
Na2 O11 2.625(17) .
Na2 O15 2.869(16) 7_665
Na2 O15 2.869(16) 4_645
Na2 O19 2.96(2) 3_545
O1 C7 1.26(2) .
O1 Ho2 2.346(11) 7_666
O2 C7 1.23(2) .
O3 C8 1.29(2) .
O4 C8 1.25(2) .
O8 C16 1.25(2) .
O8 Ho1 2.301(13) 5_675
O9 C16 1.27(2) .
O9 Ho3 2.453(12) 2_655
O10 C15 1.22(2) .
O10 Ho4 2.227(12) 7_665
O11 C15 1.26(2) .
O15 Ho3 2.321(10) 2_655
O15 Na2 2.869(16) 7_665
O15 H15 0.8498 .
O16 Ho4 2.297(12) 2_655
O16 H16 0.8500 .
O17 Ho3 2.341(9) 6_575
O17 H17 0.8500 .
O18 H18 0.8499 .
O19 Ho3 2.331(10) 6_575
O19 Na2 2.96(2) 3_455
O19 H19 0.8499 .
O20 H20 0.8499 .
O21 Ho1 2.426(19) 5_676
O21 H21 0.8501 .
O22 H22 0.8500 .
O23 H23 0.8499 .
O24 H24A 0.8498 .
O24 H24B 0.8500 .
O25 H25 0.8500 .
O26 H26 0.8500 .
O27 H27 0.8502 .
O28 H28 0.8499 .
O29 H29A 0.8500 .
O29 H29B 0.8500 .
O30 H30 0.8498 .
C1 C6 1.36(3) .
C1 C2 1.37(2) .
C1 H1 0.9500 .
C2 C3 1.39(2) .
C2 H2 0.9500 .
C3 C4 1.39(3) .
C3 C8 1.48(2) .
C4 C5 1.43(2) .
C5 C6 1.38(2) .
C5 H5 0.9500 .
C6 C7 1.49(2) .
C9 C14 1.36(2) .
C9 C10 1.41(2) .
C9 C15 1.49(2) .
C10 C11 1.36(2) .
C10 H10 0.9500 .
C11 C12 1.38(3) .
C12 C13 1.38(2) .
C12 C16 1.53(2) .
C13 C14 1.40(2) .
C13 H13 0.9500 .
C14 H14 0.9500 .
